#------------------------------------------------------------------------------
#$Date: 2015-09-21 03:45:58 +0300 (Mon, 21 Sep 2015) $
#$Revision: 158199 $
#$URL: svn://www.crystallography.net/cod/cif/2/02/01/2020125.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2020125
loop_
_publ_author_name
'Prakash, Jai'
'Schäfer, Marion C.'
'Bobev, Svilen'
_publ_section_title
;
 Synthesis and structure determination of seven ternary bismuthides:
 crystal chemistry of the RELi₃Bi₂ family (RE = La--Nd,
 Sm, Gd, and Tb)
;
_journal_coeditor_code           SK3600
_journal_issue                   10
_journal_name_full               'Acta Crystallographica Section C'
_journal_page_first
;
;
_journal_paper_doi               10.1107/S2053229615016393
_journal_volume                  71
_journal_year                    2015
_chemical_formula_iupac          'Gd Li3 Bi2'
_chemical_formula_sum            'Bi2 Gd Li3'
_chemical_formula_weight         596.03
_chemical_name_systematic
;
Gadolinium trilithium dibismuthide
;
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_symmetry_space_group_name_Hall  '-P 3 2"'
_symmetry_space_group_name_H-M   'P -3 m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            1
_cell_length_a                   4.6188(7)
_cell_length_b                   4.6188(7)
_cell_length_c                   7.328(2)
_cell_measurement_reflns_used    547
_cell_measurement_temperature    200(2)
_cell_measurement_theta_max      24.67
_cell_measurement_theta_min      2.78
_cell_volume                     135.39(5)
_computing_cell_refinement
;
SAINT (Bruker, 2007)
;
_computing_data_collection
;
APEX2 (Bruker, 2007)
;
_computing_data_reduction
;
SAINT (Bruker, 2007)
;
_computing_molecular_graphics
;
CrystalMaker (Palmer, 2007)
;
_computing_publication_material
;
publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXTL (Sheldrick, 2008)
;
_computing_structure_solution
;
SHELXS97 (Sheldrick, 2008)
;
_diffrn_ambient_temperature      200(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_measurement_device_type  'Bruker APEXII CCD'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0514
_diffrn_reflns_av_sigmaI/netI    0.0276
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_limit_l_min       -10
_diffrn_reflns_number            2067
_diffrn_reflns_theta_full        30.58
_diffrn_reflns_theta_max         30.58
_diffrn_reflns_theta_min         2.78
_exptl_absorpt_coefficient_mu    76.749
_exptl_absorpt_correction_T_max  0.3731
_exptl_absorpt_correction_T_min  0.2830
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
(SADABS; Sheldrick, 2008)
;
_exptl_crystal_colour            silver
_exptl_crystal_density_diffrn    7.310
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       irregular
_exptl_crystal_F_000             239
_exptl_crystal_size_max          0.02
_exptl_crystal_size_mid          0.02
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.567
_refine_diff_density_min         -1.451
_refine_ls_extinction_coef       0.0016(10)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method
;
SHELXTL (Sheldrick, 2008)
;
_refine_ls_goodness_of_fit_ref   1.084
_refine_ls_matrix_type           full
_refine_ls_number_parameters     9
_refine_ls_number_reflns         192
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.084
_refine_ls_R_factor_all          0.0266
_refine_ls_R_factor_gt           0.0233
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0225P)²+0.9138P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0467
_refine_ls_wR_factor_ref         0.0475
_reflns_number_gt                177
_reflns_number_total             192
_reflns_threshold_expression     I>2sigma(I)
_cod_data_source_file            sk3600sup1.cif
_cod_data_source_block           GdLi3Bi2
_cod_database_code               2020125
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_symmetry_multiplicity
Li Li1 0.3333 0.6667 0.643(5) 0.033(7) Uiso d S 1 6
Li Li2 0.0000 0.0000 0.5000 0.033(7) Uiso d S 1 12
Gd Gd1 0.0000 0.0000 0.0000 0.0099(3) Uani d S 1 12
Bi Bi1 0.3333 0.6667 0.24612(8) 0.0109(2) Uani d S 1 6
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Li Li -0.0003 0.0001 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Gd Gd -0.1653 3.9035 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
Bi1 Li1 Bi1 7_666 7_676 111.9(7)
Bi1 Li1 Bi1 7_666 7_566 111.9(7)
Bi1 Li1 Bi1 7_676 7_566 111.9(7)
Bi1 Li1 Li2 7_666 1_565 175.5(15)
Bi1 Li1 Li2 7_676 1_565 70.21(5)
Bi1 Li1 Li2 7_566 1_565 70.21(5)
Bi1 Li1 Li2 7_666 . 70.21(5)
Bi1 Li1 Li2 7_676 . 175.5(15)
Bi1 Li1 Li2 7_566 . 70.21(5)
Li2 Li1 Li2 1_565 . 107.4(8)
Bi1 Li1 Li2 7_666 1_665 70.21(5)
Bi1 Li1 Li2 7_676 1_665 70.21(5)
Bi1 Li1 Li2 7_566 1_665 175.5(15)
Li2 Li1 Li2 1_565 1_665 107.4(8)
Li2 Li1 Li2 . 1_665 107.4(8)
Bi1 Li1 Bi1 7_666 . 107.0(7)
Bi1 Li1 Bi1 7_676 . 107.0(7)
Bi1 Li1 Bi1 7_566 . 107.0(7)
Li2 Li1 Bi1 1_565 . 68.6(7)
Li2 Li1 Bi1 . . 68.6(7)
Li2 Li1 Bi1 1_665 . 68.6(7)
Bi1 Li1 Li1 7_666 7_666 55.1(3)
Bi1 Li1 Li1 7_676 7_666 123.8(5)
Bi1 Li1 Li1 7_566 7_666 123.8(5)
Li2 Li1 Li1 1_565 7_666 120.4(17)
Li2 Li1 Li1 . 7_666 53.7(4)
Li2 Li1 Li1 1_665 7_666 53.7(4)
Bi1 Li1 Li1 . 7_666 51.8(10)
Bi1 Li1 Li1 7_666 7_566 123.8(5)
Bi1 Li1 Li1 7_676 7_566 123.8(5)
Bi1 Li1 Li1 7_566 7_566 55.1(3)
Li2 Li1 Li1 1_565 7_566 53.7(4)
Li2 Li1 Li1 . 7_566 53.7(4)
Li2 Li1 Li1 1_665 7_566 120.4(17)
Bi1 Li1 Li1 . 7_566 51.8(10)
Li1 Li1 Li1 7_666 7_566 85.8(15)
Bi1 Li1 Li1 7_666 7_676 123.8(5)
Bi1 Li1 Li1 7_676 7_676 55.1(3)
Bi1 Li1 Li1 7_566 7_676 123.8(5)
Li2 Li1 Li1 1_565 7_676 53.7(4)
Li2 Li1 Li1 . 7_676 120.4(17)
Li2 Li1 Li1 1_665 7_676 53.7(4)
Bi1 Li1 Li1 . 7_676 51.8(10)
Li1 Li1 Li1 7_666 7_676 85.8(15)
Li1 Li1 Li1 7_566 7_676 85.8(15)
Bi1 Li1 Gd1 7_666 1_666 56.9(4)
Bi1 Li1 Gd1 7_676 1_666 56.9(4)
Bi1 Li1 Gd1 7_566 1_666 118.6(12)
Li2 Li1 Gd1 1_565 1_666 126.0(5)
Li2 Li1 Gd1 . 1_666 126.0(5)
Li2 Li1 Gd1 1_665 1_666 65.9(3)
Bi1 Li1 Gd1 . 1_666 134.5(4)
Li1 Li1 Gd1 7_666 1_666 98.7(5)
Li1 Li1 Gd1 7_566 1_666 173.7(14)
Li1 Li1 Gd1 7_676 1_666 98.7(5)
Bi1 Li1 Gd1 7_666 1_566 118.6(12)
Bi1 Li1 Gd1 7_676 1_566 56.9(4)
Bi1 Li1 Gd1 7_566 1_566 56.9(4)
Li2 Li1 Gd1 1_565 1_566 65.9(3)
Li2 Li1 Gd1 . 1_566 126.0(5)
Li2 Li1 Gd1 1_665 1_566 126.0(5)
Bi1 Li1 Gd1 . 1_566 134.5(4)
Li1 Li1 Gd1 7_666 1_566 173.7(14)
Li1 Li1 Gd1 7_566 1_566 98.7(5)
Li1 Li1 Gd1 7_676 1_566 98.7(5)
Gd1 Li1 Gd1 1_666 1_566 76.4(6)
Li1 Li2 Li1 7_556 7_666 107.4(8)
Li1 Li2 Li1 7_556 1_445 72.6(8)
Li1 Li2 Li1 7_666 1_445 180.0000(10)
Li1 Li2 Li1 7_556 . 179.9990(10)
Li1 Li2 Li1 7_666 . 72.6(8)
Li1 Li2 Li1 1_445 . 107.4(8)
Li1 Li2 Li1 7_556 7_566 107.4(8)
Li1 Li2 Li1 7_666 7_566 107.4(8)
Li1 Li2 Li1 1_445 7_566 72.6(8)
Li1 Li2 Li1 . 7_566 72.6(8)
Li1 Li2 Li1 7_556 1_545 72.6(8)
Li1 Li2 Li1 7_666 1_545 72.6(8)
Li1 Li2 Li1 1_445 1_545 107.4(8)
Li1 Li2 Li1 . 1_545 107.4(8)
Li1 Li2 Li1 7_566 1_545 180.0(14)
Li1 Li2 Bi1 7_556 7_666 126.2(3)
Li1 Li2 Bi1 7_666 7_666 56.4(7)
Li1 Li2 Bi1 1_445 7_666 123.6(7)
Li1 Li2 Bi1 . 7_666 53.8(3)
Li1 Li2 Bi1 7_566 7_666 126.2(3)
Li1 Li2 Bi1 1_545 7_666 53.8(3)
Li1 Li2 Bi1 7_556 1_445 53.8(3)
Li1 Li2 Bi1 7_666 1_445 123.6(7)
Li1 Li2 Bi1 1_445 1_445 56.4(7)
Li1 Li2 Bi1 . 1_445 126.2(3)
Li1 Li2 Bi1 7_566 1_445 53.8(3)
Li1 Li2 Bi1 1_545 1_445 126.2(3)
Bi1 Li2 Bi1 7_666 1_445 180.0
Li1 Li2 Bi1 7_556 7_556 56.4(7)
Li1 Li2 Bi1 7_666 7_556 126.2(3)
Li1 Li2 Bi1 1_445 7_556 53.8(3)
Li1 Li2 Bi1 . 7_556 123.6(7)
Li1 Li2 Bi1 7_566 7_556 126.2(3)
Li1 Li2 Bi1 1_545 7_556 53.8(3)
Bi1 Li2 Bi1 7_666 7_556 90.511(17)
Bi1 Li2 Bi1 1_445 7_556 89.489(17)
Li1 Li2 Bi1 7_556 . 123.6(7)
Li1 Li2 Bi1 7_666 . 53.8(3)
Li1 Li2 Bi1 1_445 . 126.2(3)
Li1 Li2 Bi1 . . 56.4(7)
Li1 Li2 Bi1 7_566 . 53.8(3)
Li1 Li2 Bi1 1_545 . 126.2(3)
Bi1 Li2 Bi1 7_666 . 89.489(17)
Bi1 Li2 Bi1 1_445 . 90.511(17)
Bi1 Li2 Bi1 7_556 . 180.0
Li1 Li2 Bi1 7_556 7_566 126.2(3)
Li1 Li2 Bi1 7_666 7_566 126.2(3)
Li1 Li2 Bi1 1_445 7_566 53.8(3)
Li1 Li2 Bi1 . 7_566 53.8(3)
Li1 Li2 Bi1 7_566 7_566 56.4(7)
Li1 Li2 Bi1 1_545 7_566 123.6(7)
Bi1 Li2 Bi1 7_666 7_566 90.511(17)
Bi1 Li2 Bi1 1_445 7_566 89.489(17)
Bi1 Li2 Bi1 7_556 7_566 90.511(17)
Bi1 Li2 Bi1 . 7_566 89.489(17)
Li1 Li2 Bi1 7_556 1_545 53.8(3)
Li1 Li2 Bi1 7_666 1_545 53.8(3)
Li1 Li2 Bi1 1_445 1_545 126.2(3)
Li1 Li2 Bi1 . 1_545 126.2(3)
Li1 Li2 Bi1 7_566 1_545 123.6(7)
Li1 Li2 Bi1 1_545 1_545 56.4(7)
Bi1 Li2 Bi1 7_666 1_545 89.489(17)
Bi1 Li2 Bi1 1_445 1_545 90.511(17)
Bi1 Li2 Bi1 7_556 1_545 89.489(17)
Bi1 Li2 Bi1 . 1_545 90.511(17)
Bi1 Li2 Bi1 7_566 1_545 180.0
Bi1 Gd1 Bi1 7 7_665 91.674(17)
Bi1 Gd1 Bi1 7 1_445 88.326(17)
Bi1 Gd1 Bi1 7_665 1_445 180.0
Bi1 Gd1 Bi1 7 . 180.0
Bi1 Gd1 Bi1 7_665 . 88.326(17)
Bi1 Gd1 Bi1 1_445 . 91.674(17)
Bi1 Gd1 Bi1 7 7_565 91.674(17)
Bi1 Gd1 Bi1 7_665 7_565 91.674(17)
Bi1 Gd1 Bi1 1_445 7_565 88.326(17)
Bi1 Gd1 Bi1 . 7_565 88.326(17)
Bi1 Gd1 Bi1 7 1_545 88.326(17)
Bi1 Gd1 Bi1 7_665 1_545 88.326(17)
Bi1 Gd1 Bi1 1_445 1_545 91.674(17)
Bi1 Gd1 Bi1 . 1_545 91.674(17)
Bi1 Gd1 Bi1 7_565 1_545 180.0
Bi1 Gd1 Li2 7 . 124.072(12)
Bi1 Gd1 Li2 7_665 . 124.072(12)
Bi1 Gd1 Li2 1_445 . 55.928(12)
Bi1 Gd1 Li2 . . 55.928(12)
Bi1 Gd1 Li2 7_565 . 124.071(12)
Bi1 Gd1 Li2 1_545 . 55.929(12)
Bi1 Gd1 Li2 7 1_554 55.928(12)
Bi1 Gd1 Li2 7_665 1_554 55.928(12)
Bi1 Gd1 Li2 1_445 1_554 124.072(12)
Bi1 Gd1 Li2 . 1_554 124.072(12)
Bi1 Gd1 Li2 7_565 1_554 55.929(12)
Bi1 Gd1 Li2 1_545 1_554 124.071(12)
Li2 Gd1 Li2 . 1_554 180.0
Bi1 Gd1 Li1 7 1_444 46.53(6)
Bi1 Gd1 Li1 7_665 1_444 101.5(4)
Bi1 Gd1 Li1 1_445 1_444 78.5(4)
Bi1 Gd1 Li1 . 1_444 133.47(6)
Bi1 Gd1 Li1 7_565 1_444 46.53(6)
Bi1 Gd1 Li1 1_545 1_444 133.47(6)
Li2 Gd1 Li1 . 1_444 134.5(4)
Li2 Gd1 Li1 1_554 1_444 45.5(4)
Bi1 Gd1 Li1 7 7_666 133.47(6)
Bi1 Gd1 Li1 7_665 7_666 78.5(4)
Bi1 Gd1 Li1 1_445 7_666 101.5(4)
Bi1 Gd1 Li1 . 7_666 46.53(6)
Bi1 Gd1 Li1 7_565 7_666 133.47(6)
Bi1 Gd1 Li1 1_545 7_666 46.53(6)
Li2 Gd1 Li1 . 7_666 45.5(4)
Li2 Gd1 Li1 1_554 7_666 134.5(4)
Li1 Gd1 Li1 1_444 7_666 180.0000(10)
Bi1 Gd1 Li1 7 1_554 101.5(4)
Bi1 Gd1 Li1 7_665 1_554 46.53(6)
Bi1 Gd1 Li1 1_445 1_554 133.47(6)
Bi1 Gd1 Li1 . 1_554 78.5(4)
Bi1 Gd1 Li1 7_565 1_554 46.53(6)
Bi1 Gd1 Li1 1_545 1_554 133.47(6)
Li2 Gd1 Li1 . 1_554 134.5(4)
Li2 Gd1 Li1 1_554 1_554 45.5(4)
Li1 Gd1 Li1 1_444 1_554 76.4(6)
Li1 Gd1 Li1 7_666 1_554 103.6(6)
Bi1 Gd1 Li1 7 7_556 78.5(4)
Bi1 Gd1 Li1 7_665 7_556 133.47(6)
Bi1 Gd1 Li1 1_445 7_556 46.53(6)
Bi1 Gd1 Li1 . 7_556 101.5(4)
Bi1 Gd1 Li1 7_565 7_556 133.47(6)
Bi1 Gd1 Li1 1_545 7_556 46.53(6)
Li2 Gd1 Li1 . 7_556 45.5(4)
Li2 Gd1 Li1 1_554 7_556 134.5(4)
Li1 Gd1 Li1 1_444 7_556 103.6(6)
Li1 Gd1 Li1 7_666 7_556 76.4(6)
Li1 Gd1 Li1 1_554 7_556 180.0
Li1 Bi1 Li1 7_666 7_676 111.9(7)
Li1 Bi1 Li1 7_666 7_566 111.9(7)
Li1 Bi1 Li1 7_676 7_566 111.9(7)
Li1 Bi1 Li1 7_666 . 73.1(7)
Li1 Bi1 Li1 7_676 . 73.1(7)
Li1 Bi1 Li1 7_566 . 73.1(8)
Li1 Bi1 Gd1 7_666 1_565 162.9(7)
Li1 Bi1 Gd1 7_676 1_565 76.5(5)
Li1 Bi1 Gd1 7_566 1_565 76.5(5)
Li1 Bi1 Gd1 . 1_565 124.072(12)
Li1 Bi1 Gd1 7_666 . 76.5(5)
Li1 Bi1 Gd1 7_676 . 162.9(7)
Li1 Bi1 Gd1 7_566 . 76.5(5)
Li1 Bi1 Gd1 . . 124.072(12)
Gd1 Bi1 Gd1 1_565 . 91.674(17)
Li1 Bi1 Gd1 7_666 1_665 76.5(5)
Li1 Bi1 Gd1 7_676 1_665 76.5(5)
Li1 Bi1 Gd1 7_566 1_665 162.9(7)
Li1 Bi1 Gd1 . 1_665 124.072(13)
Gd1 Bi1 Gd1 1_565 1_665 91.674(17)
Gd1 Bi1 Gd1 . 1_665 91.674(17)
Li1 Bi1 Li2 7_666 1_565 128.1(7)
Li1 Bi1 Li2 7_676 1_565 56.0(4)
Li1 Bi1 Li2 7_566 1_565 56.0(4)
Li1 Bi1 Li2 . 1_565 55.098(12)
Gd1 Bi1 Li2 1_565 1_565 68.974(17)
Gd1 Bi1 Li2 . 1_565 131.317(5)
Gd1 Bi1 Li2 1_665 1_565 131.317(5)
Li1 Bi1 Li2 7_666 1_665 56.0(4)
Li1 Bi1 Li2 7_676 1_665 56.0(4)
Li1 Bi1 Li2 7_566 1_665 128.1(7)
Li1 Bi1 Li2 . 1_665 55.098(12)
Gd1 Bi1 Li2 1_565 1_665 131.317(5)
Gd1 Bi1 Li2 . 1_665 131.317(5)
Gd1 Bi1 Li2 1_665 1_665 68.974(17)
Li2 Bi1 Li2 1_565 1_665 90.511(17)
Li1 Bi1 Li2 7_666 . 56.0(4)
Li1 Bi1 Li2 7_676 . 128.1(7)
Li1 Bi1 Li2 7_566 . 56.0(4)
Li1 Bi1 Li2 . . 55.098(12)
Gd1 Bi1 Li2 1_565 . 131.317(5)
Gd1 Bi1 Li2 . . 68.974(17)
Gd1 Bi1 Li2 1_665 . 131.317(5)
Li2 Bi1 Li2 1_565 . 90.511(17)
Li2 Bi1 Li2 1_665 . 90.511(17)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Li1 Bi1 7_666 2.788(11)
Li1 Bi1 7_676 2.788(11)
Li1 Bi1 7_566 2.788(11)
Li1 Li2 1_565 2.865(14)
Li1 Li2 . 2.865(14)
Li1 Li2 1_665 2.865(14)
Li1 Bi1 . 2.91(4)
Li1 Li1 7_666 3.39(5)
Li1 Li1 7_566 3.39(5)
Li1 Li1 7_676 3.39(5)
Li1 Gd1 1_666 3.74(3)
Li1 Gd1 1_566 3.74(3)
Li2 Li1 7_556 2.865(14)
Li2 Li1 7_666 2.865(14)
Li2 Li1 1_445 2.865(14)
Li2 Li1 7_566 2.865(14)
Li2 Li1 1_545 2.865(14)
Li2 Bi1 7_666 3.2515(6)
Li2 Bi1 1_445 3.2515(6)
Li2 Bi1 7_556 3.2515(6)
Li2 Bi1 . 3.2515(6)
Li2 Bi1 7_566 3.2515(6)
Li2 Bi1 1_545 3.2515(6)
Gd1 Bi1 7 3.2193(5)
Gd1 Bi1 7_665 3.2193(6)
Gd1 Bi1 1_445 3.2193(6)
Gd1 Bi1 . 3.2193(6)
Gd1 Bi1 7_565 3.2193(6)
Gd1 Bi1 1_545 3.2193(6)
Gd1 Li2 1_554 3.6640(10)
Gd1 Li1 1_444 3.74(3)
Gd1 Li1 7_666 3.74(3)
Gd1 Li1 1_554 3.74(3)
Gd1 Li1 7_556 3.74(3)
Bi1 Li1 7_666 2.788(11)
Bi1 Li1 7_676 2.788(11)
Bi1 Li1 7_566 2.788(11)
Bi1 Gd1 1_565 3.2193(6)
Bi1 Gd1 1_665 3.2193(6)
Bi1 Li2 1_565 3.2515(6)
Bi1 Li2 1_665 3.2515(6)

_cod_database_fobs_code 2020125
